Mathematical Modeling of Optical Radiation Emission as a Function of Welding Power during Gas Shielded Metal Arc Welding
Abstract Arc welding is accompanied by intense optical radiation emission that can be detrimental not only for the welder himself but also for people working nearby or for passersby. Technological progress advances continuously in the field of joining, so an up-to-date radiation database is necessary. Additionally, many literature irradiance data have been measured for a few welding currents or for parts of the optical spectral region only. Within this paper, a comprehensive study of contemporary metal active gas, metal inert gas, and cold metal transfer welding is presented covering optical radiation emission from 200 up to 2,700 nm by means of (spectro-) radiometric measurements. The investigated welding currents range from 70 to 350 A, reflecting values usually applied in industry. Based upon these new irradiance data, three mathematical models were derived in order to describe optical radiation emission as a function of welding power. The linear, exponential, and sigmoidal emission models depend on the process variant (standard or pulsed) as well as on the welding material (mild and stainless steel, aluminum). In conjunction with the corresponding exposure limit values for incoherent optical radiation maximum permissible exposure durations were calculated as a function of welding power. Typical times are shorter than 1 s for the ultraviolet spectral region and range from 1 to 10 s for visible radiation. For the infrared regime, exposure durations are of the order of minutes to hours. Finally, a validation of the metal active gas emission models was carried out with manual arc welding.
Spectra of optical radiation from welding arcs.
It is important to determine spectra of optical radiation from light sources at workplaces, because they usually emit lights of various wavelengths simultaneously and these differ in their degree of harmfulness. Spectra of optical radiation (wavelength range: 200-1, 000 nm) from the arc of various arc welding processes were measured, using a multichannel detector system. For each process, a stable relative spectrum (a shape of the spectrum) was obtained in spite of the fluctuations in intensity. The relative spectrum is determined mainly by the welding material, such as steel or aluminum, regardless of the other parameters. Especially, it is independent of the diameter of wire, arc current and arc voltage, which have an influence only on the absolute intensity of the radiation.
Hygroscopic Expansion of some Casting Investments
CREDIT is generally given to Taggart1 for introducing the cast gold inlay to the dental profession. Although he realized that gold shrinks when cooled from molten state to solid state of room temperature, the investment available to him did not supply sufficient compensation. In 1910, Van Horn2 published a paper dealing with a method by which he obtained the compensation by means of wax expansion. The next major research in connection with this problem was the work of Coleman3 at the National Bureau of Standards. He determined the gold shrinkage to be 1.25 per cent and presented a casting technic with compensation values of quantitative nature. The total compensation for the gold shrinkage was obtained by the combination of the setting and thermal expansion of the mold. This procedure is the general practice followed at the present time for compensation. There are some disadvantages to this method. Skinner has indicated the difficulty of obtaining smooth castings and the improper compensation for the casting shrinkage.4 It has been found by Hollenback5 and Scheu6a that castings made at a high temperature are rougher than those made at a low temperature (450° C.), depending upon the great difference in thermal expansion between plaster of Paris and silica, which causes a poor union of the fine particles. This may also result in friability and there may be some warpage due to the differential expansion. A method which provides sufficient compensation at a low mold temperature is the hygroscopic casting technic.b Wilson7 showed that certain plasters expand as much as 0.0044 inch to the inch by taking up moisture from the air. With this information at hand, Scheula, b tested some commercial investment to determine what results the addition of moisture would have. He found6b: (1) All of the casting investments that were tested expanded. (2) The thicker the mix, the greater the expansion. (3) A mix with hot water expanded more than one with cold water. (4) The time at which the mix is placed in the water is of great importance. It was found that if the mix is placed in the water early, it would not expand so much as when placed in a little later. It was also found that if the mix was placed in the water after a certain time, it could not expand to the maximal amount. (5) The temperature of the water in which the mix is placed is important, for two reasons; (a) the temperature of the water controls slightly the expansion of the investment, and (b) water at a temperature of 1000 F. slightly softens the wax pattern so that the fine margins are not marred while expansion is taking place. The mix should remain in the water at least 20 minutes to obtain the full expansion, after which time no further expansion is obtained.